### UNIVERSITAT POLITÈCNICA DE CATALUNYA

### DEPARTAMENT D’ENGINYERIA QUÍMICA

**APPLICATION OF MOLECULAR **

**SIMULATION TECHNIQUES TO THE **

**DESIGN OF NANOSYSTEMS **

### Francisco Rodríguez Ropero

**Advisors:**

### Dr.Carlos Alemán Llansó y Dr. David Zanuy Gómara

**OBJECTIVES**

(1) Improve the stability of tubular nanodevices based on highly regular β-helical motifs excised from naturally occurring proteins by replacing targeted natural residues by conformationally constrained synthetic amino acids.

(2) Model and characterize a dendronized polymethacrylate carrying second generation chiral 4-aminoproline-based dendrons and a thiophene based dendronized polymer in order to explain, in basis of their structure, the extraordinary stiffness of the first and the great conductivity exhibited by the latter in previous experimental studies.

(3) Study of the interactions of thiophene based conducting polymers. The interaction of these polymers with the solvent medium as well as their intermolecular interactions such as π-stacking interactions play a key role when designing new devices based on conducting polymers.

(4) Exploit the intrinsic tubular geometry of natural motifs extracted from certain proteins together with the ability of π-conjugated systems to promote charge transfer to model a tubular electronic conductor based on natural peptide sequences by replacing natural amino acids by synthetic amino acids owning an aromatic side chain.

(5) Study of the role played by the solvent molecules in the actuation mechanism in the molecular actuator poly(calix[4]arene bis-bithiophene) by the examination of the structure and dynamics of the dichloromethane solvent around the calix[4]arene units.

**ABBREVIATIONS **

1hv9 residues 296-329 of N-acetylglucosamine 1-phosphate uridyltransferase
GlmU, C-terminal domain from *Eschericia coli*

1krr Residues 131-165 of the chain A from the *Escherichia coli* galactoside
acetyltransferase

Ac3c 1-aminocyclopropane-1-carboxylic acid

Ac4c 1-aminocyclobutane-1-carboxylic acid

Ac5c 1-aminocyclopentane-1-carboxylic acid

Ac6c 1-aminocyclohexane-1-carboxylic acid

Acnc 1-aminocycloalkane-1-carboxylic acids

Aib _{-aminoisobutyric acid }
AIBN _{2,2’-azobisisobutyronitrile}

AIMI _{Aromatic Intermolecular Interaction Model }
AM1 Austin Model number 1

B3LYP Becke’s three parameter hybrid functional with the Lee, Yang and Parr expression.

Boc *tert-*butoxycarbonyl

BSSE Basis Set Superposition Error

c3Dip 1-amino-2,2-diphenyl-cyclopropanecarboxylic acid

CC Coupled Cluster

CCSD(T) Coupled cluster singles, doubles and triples method being the contribution of triple excitations represented in an approximate way

CD Circular Dichroism

CP Counterpoise DFT Density Functional Theory

DSC Differential Scanning Calorimetry Dg Diphenylglycine

ESP Electrostatic potential

FF Force Field

GGA Generalised Gradient Approximation

Ĥ Hamiltonian operator

HF Hartree Fock

HOMO Highest Occupied Molecular Orbital

**iv**

KT Koopman’s Theorem

LCAO Linear Combination of Atomic Orbitals LDA Local Density Approximation

LSCF Local Self-Consistent Field

LSDA Local Spin Density Approximation LUMO Lowest Unoccupied Molecular Orbital

MD Molecular Dynamics

MEP Molecular Electrostatic Potential MGn nth Generation monomer (dendron)

MM Molecular Mechanics

MP Møller Plesset

NA9PH 9-(2,3-dihydro-2-phenyl-1H-benz[e]inden-1-ylidene)-9H-fluorene NA9PH(S) NA9PH Singlet state

NA9PH(T) NA9PH Triplet state

NPT Isobaric-isothermal ensemble

NVT Canonical ensemble

OR Optical Rotation

PCM Polarizable Continuum Model PDB Protein Data Bank

PGn nth Generation polymer (dendronized polymer)

PM3 Parameterized Model number 3 PME Particle Mesh Ewald

PMF Potential Mean Force

PMMA Poly(methyl methacrylate)

QM Quantum Mechanics

QM/MM Quantum mechanics/Molecular mechanics RESP Restrained Electrostatic Potential RMSD Root Mean Square Deviation

RMSF Root Mean Square Fluctuation

r.u. Repeat Unit

SCF Self Consistent Field

SCRF Self Consistent Reaction Field

SE Semiempirical

SLBO Strictly Localized Bond Orbitals

STO Slater Type Orbital

TD Time-dependent Tie β-3-thienylalanine

UB3LYP Unrestricted B3LYP UHF Unrestricted Hartree Fock

UMP2 Unrestricted MP2

UPM3 Unrestricted PM3

wt Wild type

ZPVE Zero-Point Vibrational Energies

Ala -Alanine

**TABLE OF CONTENTS **

**1.**

**Introduction ... 1**

1.1. A brief description of nanotechnology: history and current state ... 3

1.2. Presence of nanotechnology: applications... 5

1.3. Role of Computational Chemistry in the development of nanodevices ... 7

1.4. References ... 10

**2.**

**Methodology...15**

2.1. Computational chemistry... 17

2.2. Quantum Mechanical Methods... 18

2.2.1. Hamiltonian operator... 18

2.2.2. Basis sets ... 19

2.2.3. Closed-shell and open-shell systems ... 21

2.2.4. Ab initio calculations... 21

2.2.5. Semiempirical calculations... 23

2.2.6. Density Functional Theory calculations ... 24

2.2.7. Solvent effects ... 25

2.3. Molecular dynamics simulations... 27

2.3.1. Force-Field ... 27

2.3.2. Mathematical model of molecular dynamics... 28

2.3.3. Thermodynamic ensembles ... 29

2.3.4. Periodic boundary conditions and Particle Mesh-Ewald Summation ... 30

2.4. QM/MM calculations ... 31

2.5. References ... 33

**3.**

**Nanotubes based on natural peptide sequences ...37**

3.1. Testing β–helix terminal coils stability by targeted substitutions with non-proteogenic amino acids: A Molecular Dynamics study... 39

3.1.1. Introduction ... 39

3.1.2. Survey of Synthetic Amino Acids... 43

3.1.3. Methods ... 44

3.1.4. Results and discussion... 47

**viii**

3.1.6. References ... 57

3.2. Stability of tubular structures based on β-helical proteins: self-assembled versus polymerized nanoconstructs and wild-type versus mutated sequences... 60

3.2.1. Introduction ... 60

3.2.2. Description of the β-helical building blocks and the Ac5c synthetic residue………. 62

3.2.3. Methods ... 63

3.2.4. Results and discussion... 66

3.2.5. Conclusions ... 79

3.2.6. References ... 80

3.3. Application of 1-aminocyclohexane carboxylic acid to protein nanostructure computer design... 83

3.3.1. Introduction ... 83

3.3.2. Methods ... 85

3.3.3. Results and discussion... 88

3.3.4. Conclusions ... 104

3.3.5. References ... 106

**4.**

**Dendronized polymers ...109**

4.1. A rigid, chiral, dendronized polymer with a thermally stable, right-handed helical conformation,... 111

4.1.1. Introduction ... 111

4.1.2. Computational methods... 112

4.1.3. Results and discussion... 114

4.1.4. Conclusions ... 126

4.1.5. References ... 128

4.2. Helical dendronized polymers carrying chiral 4-aminoproline second-generation dendrons: Atomistic view and driving forces... 132

4.2.1. Introduction ... 132

4.2.2. Methods ... 134

4.2.3. Results and discussion... 136

4.2.4. Conclusions ... 149

4.3. Electronic characterization of all-thiophene conducting dendrimers: Molecules

and assemblies ... 153

4.3.1. Introduction ... 153

4.3.2. Methods ... 155

4.3.3. Results and discussion... 158

4.3.4. Conclusions ... 167

4.3.5. References ... 169

**5.**

**Theoretical study of **

**π**

**-conjugated systems ...173**

5.1. Solvation of 2,2’-bithiophene: influence of the first solvation shell in the properties of π-conjugated systems ... 175

5.1.1. Introduction ... 175

5.1.2. Methods ... 176

5.1.3. Results and discussion... 177

5.1.4. Conclusions ... 183

5.1.5. References ... 184

5.2. *Ab initio* calculations on π-stacked thiophene dimer, trimer and tetramer:
structure, interaction energy, cooperative effects and intermolecular electronic
parameters... 185

5.2.1. Introduction ... 185

5.2.2. Computational methods... 187

5.2.3. Results and discussion... 189

5.2.4. Conclusions ... 201

5.2.5. References ... 202

5.3. On the π-dimerization of oxidized thiophene oligomers: a theoretical investigation... 205

5.3.1. Introduction ... 205

5.3.2. Computational methods... 206

5.3.3. Results and discussion... 207

5.3.4. Conclusions ... 216

5.3.5. References ... 217

5.4. Modeling an electronic conductor based on natural peptide sequences... 219

5.4.1. Introduction ... 219

**x**

5.4.3. Results and discussion... 223

5.4.4. Conclusions ... 232

5.4.5. References ... 233

**6.**

**Molecular actuators and sensors based on **

**conducting polymers ...237**

6.1. Molecular dynamics of a calix[4]arene-containing polymer in dichloromethane solution: Ability of the solvent molecules to fill the cavity of the macrocycle... 239

6.1.1. Introduction ... 239

6.1.2. Methods ... 241

6.1.3. Results and discussion... 243

6.1.4. Conclusions ... 253

6.1.5. References ... 255

6.2. Sensing mechanism of calix[4]arene-substituted polythiophene ion receptor: Effects of the selectivity on the molecular rigidity... 256

6.2.1. Introduction ... 256

6.2.2. Methods ... 257

6.2.3. Results and discussion... 259

6.2.4. Conclusions ... 266

6.2.5. References ... 267

6.3. Controlled isomerization of a light-driven molecular motor: A theoretical study 269 6.3.1. Introduction ... 269

6.3.2. Methods ... 271

6.3.3. Results and discussion... 273

6.3.4. Conclusions ... 285

6.3.5. References ... 286

**7.**

**Summary and discussion of the results ...291**

**1.1.A brief description of nanotechnology: history and current state **

Nanotechnology is a multidisciplinary branch of science and technology that involves a wide range of different fields such as chemistry, materials science, physics or chemical engineering whose goal is the production of new functional materials and devices through the control of their organization at the atomic and molecular scale.

What differences nanotechnology from traditional chemistry and physics can be summarized in three points:1

Analysis and control of the matter at the atomic and molecular level focusing in individual atoms.

The appearance of novel physical properties because of the nanoscopic dimensions.

The possibility of generating new complex functional systems with novel properties.

Professor Norio Taniguchi defined for the first time the term “Nanotechnology” in 1974 as the production technology to get the extra high accuracy and ultra fine dimensions, i.e. the preciseness and fineness on the order of 1 nanometer.2 But the concept of nanotechnology is much older. Specifically, it dates back 50 years ago when the Nobel laureate Richard Feynman gave his famous lecture entitled “There’s Plenty of Room at the Bottom” at the annual meeting of the West Coast Section of the American Physical Society held at the California Institute of Technology. In such lecture Richard Feynman envisioned the possibility of building extremely small robots, information storage devices or motors by maneuvering individual atoms.3 In spite of the revolutionary ideas exposed by Richard Feynman it was not until late 1970s and early 1980s when nanotechnology gained a certain attention in the scientific community.4

Dr. K. Eric Drexler is considered the pioneer of modern molecular nanotechnology. He borrowed the word from Prof. Taniguchi and the primordial ideas of Prof. Feynman to explain the possibility of building machines on the scale of molecules, nanomotors, robot arms or nanocomputers.5 Drexler advanced the proposal that the molecular machinery found in living systems demonstrates the feasibility of doing advanced molecular engineering to produce complex, artificial molecular machines.6

1. INTRODUCTION _{4}

very first time.7 Many progresses were done in the following years such as the discovery of the buckminsterfullerene molecule,8 the invention of the Atomic Force Microscope (AFM),9 the first engineered protein10 or the finding of the carbon nanotubes.11

All these advances in molecular engineering encouraged scientists to set up formal organizations, being the first one the Foresight Institute founded by K. Eric Drexler and Christine Peterson in 1986 in Palo Alto, California. Foresight Institute together with the Global Business Network sponsored the first comprehensive conference on nanotechnology held in Palo Alto in October 1989 where a broad range of technologies that contribute to nanotechnology as well as several perspectives for the future were presented.12

In early 90s it was clear that nanotechnology would play a key role in the development of the future world and first national funding programs in nanotechnology arose in Japan13 and in the USA,14 which summed up $185 million into a project over 10 years and $40 million respectively. Investment in nanotechnology has increased exponentially in the last years. According to the “The Global Market for Nanotechnology” edited in November 2008 by Nanoposts (University of Stirling, Innovation Park) worldwide investment in nanotechnology research in 2008 was approximately $12.3 billion, $6.7 billion coming from public funding programs, being the U.S.A., the E.U. and Japan on the top of the list. In this sense the 2009 North American Budget provides $1.5 billion for the National Nanotechnology Initiative (NNI).15 The Seventh Research Framework Program (FP7) of the E.U. includes specific areas devoted to nanosciences and nanotechnologies with a €3.5 billion portion of the budget to be invested from 2007 to 2013.16 Public investment in Japan rose up to $1.06 billion in 2007.17

The current trend is the mixture of nanotechnology and supramolecular chemistry, i.e. using the preciseness of the first with concepts such as hydrogen bonding, van der Waals interactions or π-π interactions –leading to molecular self-assembly– of the latter to build more complex structures.20

**1.2.Presence of nanotechnology: applications **

As previously stated nanotechnology has jumped from research laboratories to our daily life and today, according to the Project on Emerging Nanotechnologies organized by the Pew Charitable Trust and the Woodrow Wilson International Center for Scholars, the number of products on the market that incorporate nanotechnology is steadily increasing. At present more than 800 manufacturer-identified nanotechnology-based consumer products are available on the market. They include numerous cosmetics, electronic devices, hardware utilities, silver based anti-microbial products, coatings or food additives just to mention few examples.21 Let us briefly summarize some actual trends and uses of nanotechnology in some fields.

*Electronics and computer science *

1. INTRODUCTION _{6}

*Biomedicine *

The potential applications of nanotechnology for diagnosis, prevention, and treatment of diseases are currently very broad. Nanotechnology applied to medical diagnosis has a potentially higher sensitivity and selectivity than classical methods.19 Regarding diagnosis several improvements have been done up to date like the development of antibody-based microfluidics system to detect different cancers,27 microfluidic chip cells for the detection of allergic responses,28 nanosensors,29 quantum dots for investigating cells or low abundance antigens30 or metallic and semiconductor nanoclusters and nanopowders as markers in nuclear imaging techniques.31 Nanotechnology has greatly aided the development of new drug delivery systems such as nanovectors,32 liposomal drug carriers,33 dendronized polymers34 or other polymer based delivery systems.35 Nanotechnology has also enhanced the scope of regenerative medicine. Some examples of the utilization of nanotechnology in the manipulation of stem cells,36 in tissue engineering37 or regeneration within the central nervous system38 are reported.

*Other applications *

The bearing of nanotechnology applications is extremely wide and ranges – besides electronics and biomedicine – from catalysis39 to cosmetics.40 Under a catalyst point of view the two major improvements stemmed from nanotechnology are the use of supported metal nanoparticles and the tuning of the catalyst surface at the atomic level.

These solutions have helped the development of high activity and selectivity catalysts. Nanotechnology also offers new horizons and possibilities in water treatment. Development of nanostructured catalytic membranes, nanosorbents, nanocatalysts and bioactive nanoparticles for treatment, purification and disinfection of surface water, groundwater and water contaminated by toxic metal ions is widely reported in the literature.41 Beyond all these previously stated applications nanotechnology has an incipient presence in the development of machine tools, insulators, motor vehicles and aircrafts, batteries, high resolution screens, light-emitting diodes or molecular actuators, just to mention some examples.42

**1.3.Role of Computational Chemistry in the development of nanodevices **

Modeling and theory are becoming vital to designing and improving nanodevices. The
intrinsic nature of nano and supramolecular scale that involves tens, hundreds and
thousands of atoms makes computational chemistry the perfect ally to design new
devices and predict their properties. Computational chemistry provides the perfect tools
to describe the electronic structure and the dynamic behavior as well as the properties
derived from them through quantum mechanics and classical mechanics formalisms.
Quantum Mechanics (QM) offer the most accurate description of the matter as it
describes its fundamental behavior at the atomic and molecular level. The use of QM
requires solving Schrödinger equation using some approximations, for instance, *ab *
*initio* or Density Functional Theory (DFT) methods. Because of the computational
expensiveness of QM methods, QM is in practice only applicable to small systems, i.e.
few dozens of atoms.

Classical mechanics or Molecular Mechanics (MM) concerns the use of simple potential-energy functions such as Coulombic potentials or harmonic oscillators to model molecular systems. In spite of not being as rigorous as quantum mechanics, MM approaches allow the inclusion of a bigger quantity of atoms describing the whole system in a reliable manner. MM approaches are widely applied in molecular structure refinement, Molecular Dynamics (MD) simulations, Monte Carlo simulations and ligand-docking simulations. A more detailed description of QM and MM based methods is included in the chapter devoted to Methodology.

pseudo-1. INTRODUCTION _{8}

atoms to represent groups of atoms. Pseudo-atoms must be parameterized so that they can reproduce as much as possible the experimental data available or the results derived from all atom classical simulations.

Since the first simulation of a protein in 197643 computational chemistry has become an essential tool in protein design,44 polymer science,45 nano-science,46 drug design47 or drug delivery systems design.48

QM calculations are useful to determine properties derived from the electronic structure such as charge density, spin density, electronic affinity, ionization potential or band-gap as well as an insight of supramolecular interactions.49 QM calculations can also provide the necessary data to set a force field for MM calculations, i.e. the functional form and parameter sets used to define the potential energy of a classical system of particles.50

The amount of examples available in the bibliography of the utilization of computational chemistry to study nanodevices is really vast so only a brief survey is given, emphasizing in systems that are similar to those presented in this thesis. Several

papers where MD simulations have been employed to model and characterize different
kinds of nanotubes can be found in the literature, being carbon nanotubes and their
derivatives the most studied ones.46 Thus, there are studies ranging from the
determination of their structure and mechanical properties51 to the diffusion of different
molecules through them or derivatives of them.46,52 Peptide based nanotubes are gaining
a certain attention due to their applicability in biomedicine as drug carriers and
nanowires.53,54,55 *In silico* methods have helped the design of new and more efficient
drug and gene delivery systems predicting their required composition, geometry,
dimensions and correct dosage.56 One of the most promising families of drug delivery
systems is that concerning dendronized polymers.57 Both experimental and
computational research in nanoactuators and nanosensors are widely reported in the
literature. Among them, those based in conducting polymers are flourishing because of
their great transport properties, electrical conductivity or rate of energy migration which
provide amplified sensitivity in nanosensors and a rapid response in nanoactuators.58,59
Combining QM and MM based methods provides a good outlook of the mechanisms
that rule the sensory and actuation behavior of these devices.60,61

1. INTRODUCTION _{10}

**1.4.References **

[1] Theis T., Parr D., Binks, P., Ying J., Drexler K.E., Schepers E., Mullis K., Bai C.,
Boland J.J., Langer R., Dobson, P., Rao C.N.R., Ferrari, M. *Nat. Nanotechnol.*, **2006**, *1*,
8.

[2] Taniguchi N. “On the Basic Concept of Nano-Technology”, **1974**, *Proc. Intl. Conf. *
*Prod. *Part II, Japan Society of Precision Engineering, Tokyo.

[3] Feynman R. P. *Engineering and Science*, **1960**, *23*, 22.

[4] Drexler K.E. “Nanosystems: Molecular Machinery, Manufacturing, and
Computation”, **1992**, John Wiley & Sons Inc., New York.

[5] Drexler K.E. “Engines of Creation: The Coming Era of Nanotechnology”, **1986**,
Anchor Books, New York.

[6] Drexler K.E. *Proc. Natl. Acad. Sci.*, **1981**, *78*, 5275.

[7] Binning G., Rohrer H., Gerber C., Weibel, E. *Phys. Rev. Lett.*, **1982**, *49*, 57.

[8] Kroto H.W., Heath J.R., O'Brien S.C., Curl R.F., Smalley R.E. *Nature*, **1985**, *318*,
162.

[9] Binning G., Quate C.F., Gerber C. *Phys. Rev. Lett.*, **1987**, *56*, 930.
[10] Ho S.P., DeGrado W.F. *J. Am. Chem. Soc.*, **1987**, *109*, 6751.
[11] Ijima S., Ichihashi T. *Nature*, **1993**, *363*, 603.

[12] Crandall B.C., ed. “Nanotechnology: molecular speculations on global abundance”,

**1996**, The MIT Press, Cambridge, Massachusets.
[13] Swinbanks D. *Nature*, **1991**, *352*, 650.
[14] Amato I. *Science*, **1991**, *254*, 1302.

[15] “National Nanotechnology Initiative FY2009 Budget and Highlights”: http://www.nano.gov/NNI_FY09_budget_summary.pdf

[16] CORDIS: Nanotechnology: EU Funding:

http://cordis.europa.eu/nanotechnology/src/eu_funding.htm

[17] Nordan M.M. “Change Required for the National Nanotechnology Initiative as
Commercialization Eclipses Discovery”, **2008**, Lux Research Inc.

[18] Lu W., Lieber C.M. *Nat. Nanotechnol.*, **2007**, *6*, 841.

[19] Riehemann K., Schneider S.W., Luger T.A., Godin B., Ferrari M., Fuchs H.

*Angew. Chem. Int. Ed.*, **2009**, *48*, 872.

[21] Project on Emerging Nanotechnologies, Woodrow Wilson International Center for
Scholars. **2009**. A Nanotechnology Consumer Products Inventory:

http://www.nanotechproject.org/inventories/consumer

[22] Chen Y., Jung G-Y., Ohlberg D.A.A., Li X., Stewart D.R., Jeppesen J.O., Nielsen
K.A., Stoddart J.F., Williams R.S. *Nanotechnology*, **2003**, *14*, 462.

[23] Szaciłowski K. *Chem. Rev.*, **2008**, *108*, 3481.

[24] Strukov D.B., Likharev K.K. *Nanotechnology*, **2005**, *16*, 888.
[25] Strukov D.B., Likharev K.K. *Nanotechnology*, **2005**, *16*, 137.
[26] Jo S.H., Kim K-H., Lu W. *Nano. Lett.*, **2009**, *9*, 870.

[27] Du Z., Colls N., Cheng K.H., Vaughn M.W., Gollahon L. *Biosens. Bioelectron.*,

**2006**, *21*, 1991.

[28] Matsubara Y., Murakami Y., Kobayashi M., Morita Y., Tamiya E. *Biosens. *
*Bioelectron.*, **2004**,* 19*, 741.

[29] Fritz J., Baller M. K., Lang H. P., Rothuizen H., Vettiger P., Meyer E., Guntherodt
H., Gerber C., Gimzewski J. K. *Science*, **2000**, *288*, 316.

[30] Alivisatos A. P., Gu W., Larabell C. *Annu. Rev. Biomed. Eng.*, **2005**, *7*, 55.
[31] Kinge S., Crego-Calama M., Reinhoudt D. N. *ChemPhysChem*, **2008**, *9*, 20.

[32] Sakamoto J., Annapragada A., Decuzzi P., Ferrari M. *Expert Opin. Drug Delivery*,

**2007**, *4*, 359.

[33] Torchilin V. P. *Nat. Rev. Drug Discovery*, **2005**, *4*, 145.

[34] Costantino L., Gandolfi F., Bossy-Nobs L., Tosi G., Gurny R., Rivasi F., Vandelli
M.A., Forni F. *Biomaterials*, **2006**, *27*, 4635.

[35] Desai N., Trieu V., Yao Z., Louie L., Ci S., Yang A., Tao C., De T., Beals B.,
Dykes D., Noker P., Yao R., Labao E., Hawkins M., Soon-Shiong P. *Clin. Cancer Res.*,

**2006**, *12*, 1317.

[36] Solanki A., Kim J.D., Lee K.B. *Nanomedicine*, **2008**, *3*, 567.
[37] Zhang L.J., Webster T.J. *Nano Today*, **2009**, *4*, 66.

[38] Tysseling-Mattiace V. M., Sahni V., Niece K. L., Birch D., Czeisler C., Fehlings
M. G., Stupp S. I., Kessler J. A. *J. Neurosci.*, **2008**, *28*, 3814.

[39] Zecchina A., Groppo E., Bordiga S. *Chem. Eur. J.*, **2007**, *13*, 2440.

[40] Nohynek G.J., Lademann J., Ribaud C., Roberts M.S. *Crit. Rev. Toxicol.*, **2007**, *37*,
251.

1. INTRODUCTION _{12}

[42] Wilson M., Kannangara K., Smith G., Simmons M., Raguse B. “Nanotechnology:
Basic Science and Emerging Technologies”, **2002**, Chapman & Hall/CRC, Boca Raton.
[43] McCammon J.A., Gelin B.R., Karplus M. *Nature*, **1977**, *267*, 585.

[44] Adcock S.A., McCammon J.A. *Chem. Rev.*, **2006**, *106*, 1589.
[45] Kremer K. *Macromol. Chem. Phys.*, **2003**, *204*, 257.

[46] Rafii-Tabar H. *Phys. Rep.-Rev. Sec. Phys. Lett.*, **2004**, *390*, 235.

[47] Jenwitheesuk E., Horst J.A., Rivas K.L., Van Voorhis W.C., Wesley C., Samudrala
R. *Trends Pharmacol. Sci.*, **2008**, *29*, 62.

[48] Arifin D.Y., Lee L.Y., Wang C.H. *Adv. Drug Deliv. Rev.*, **2006**, *58*, 1274.

[49] Min S.K., Lee E.C., Lee H.M., Kim D.Y., Kim D., Kim K.S. *J. Comput. Chem.*,

**2007**,* 29*, 1208.

[50] Cornell W.D., Cieplak P., Bayly C.I., Gould I.R., Merz K.M. Jr., Ferguson D.M.,
Spellmeyer D.C., Fox T., Caldwell J.W., Kollman P.A. *J. Am. Chem. Soc.*, **1995**, *117*,
5179.

[51] Alexiadis A., Kassinos S. *Chem. Rev.*, **2008**, *108*, 5014.
[52] Liu Y.C., Wang Q. *Phys. Rev. B*, **2005**, *72*, 085420.

[53] Teranishi M., Okamoto H., Takeda K., Nomura K., Nakano A., Kalia R.K.,
Vashishta P., Shimojo F. *J. Phys. Chem. B*, **2009**, *113*, 1473.

[54] Haspel N., Zanuy D., Alemán C., Wolfson H., Nussinov R. *Structure*, **2006**, *14*,
1137.

[55] Haspel N., Zanuy D., Zheng J., Alemán C., Wolfson H., Nussinov R. *Biophys. J.*,

**2007**, *93*, 245.

[56] Haworth I.S. *Adv. Drug Deliv. Rev.*, **2006**, *58*, 1271.
[57] Gibson S.E., Rendell J.T. *Chem. Commun.*, **2008**, 922.
[58] Swager, T.M. *Acc. Chem. Res.*, **1998**, *31*, 201.

[59] Otero T.F., Cortés M. *Adv. Mater.*, **2003**, *15*, 279.

**2.1.Computational chemistry **

All the work included in the present thesis has been performed using computational methods. Computational chemistry can be roughly defined as a set of theoretical methodologies for investigating chemical problems on a computer.Thus progresses in computational chemistry have befallen closely with the headways in computer science. As previously stated computational chemistry faces chemical problems according to two formalisms: QM and MM. QM calculations require a big amount of CPU time and, since it increases exponentially with the size of the system, only small systems are affordable by using QM formalism. Bigger systems are studied using MM methods.

Since each work presented in this thesis contains a specific section devoted to the methods, only a general overview of QM based methods and MM is presented in this chapter. A deeper description of these methods can be found in many text books, for instance “Computational Chemistry: Introduction to the Theory and Applications of Molecular and Quantum Mechanics” by Errol Lewars.1

2. METHODOLOGY _{18}

**2.2.Quantum Mechanical Methods **

Quantum mechanics deals with the motion of electrons under the influence of the electromagnetic force exerted by nuclear charges. Most QM methods assume that nuclei and electron are distinguished from each other and both electron and electron-nucleus interactions are explicitly described. These interactions, which are ruled by nuclear and electron charges and electron motions, determine the spatial distribution of nuclei and electrons and their energies. Electrons are considered as wave-like particles, which are represented by a set of wave functions obtained by solving the Schrödinger equation (equation 2.1.):

ψ

E

ψ

Hˆ (2.1.)

where*H*ˆ is the Hamiltonian operator containing the kinetic and potential energy of the

nuclei and electrons, *E* is the energy of the system and *ψ* is the wave function that
describes the molecular orbitals.

Solving a QM problem implies solving the Schrödinger equation, which is only
affordable by using some approximations. In this sense *Ab initio *calculations,
semiempirical calculations and calculations based in the Density Functional Theory
(DFT) are extensively widespread to solve QM problems.

**2.2.1.** **Hamiltonian operator **

Hamiltonian (*H*ˆ ) is defined as the operator that contains all the operations associated

with the kinetic and potential energies. The general expression of the Hamiltonian for a system with M nuclei and N electrons described respectively by position vectors RA and

ri is given in equation 2.2.

###

###

###

###

###

M 1 A M A B AB B A N 1 i N 1 j ij M 1 A N 1 i M 1 A iA A 2 A A 2 i N 1 i R Z Z r 1 r Z 2M 1 2 1Hˆ (2.2.)

where *MA* is the relation of the mass of the nucleus A with respect to the mass of the

electron, *ZA* is the atomic number of the nucleus A and

2 i

and _{} 2A _{ are the Laplace }

nucleus *A *respectively. In equation 2.2. the first two terms are related to the kinetic
energy of the electrons and nuclei respectively, the third term defines the electrostatic
attraction between nuclei and electrons and the last two terms are, respectively, the
electrostatic repulsion between electrons and nuclei. Taking into account the
Born-Oppenheimer approximation, which states that nuclei in a molecule are stationary with
respect to the electrons because of their higher mass, the second and fifth terms of
equation 2.2. can be neglected. These simplifications lead to the so called electronic
Hamiltonian (equation 2.3.).

###

###

###

N 1 i M 1 A N 1 i N 1 j ij iA A 2 i N 1 i el r 1 r Z 2 1Hˆ (2.3.)

**2.2.2.** **Basis sets **

Molecular orbitals can be represented as linear combinations of m basis functions (equation 2.4.).2

s m

1 s

si i c φ

ψ

###

(2.4.)

where *ψi* is the ith molecular orbital, *φs* is the sth basis function and *csi* are weighting

coefficients that must be adjusted to get the best molecular orbital.

This approach to generate molecular orbitals is called Linear Combination of Atomic Orbitals (LCAO) in spite that these basis functions are not necessarily atomic orbitals but any set of mathematical functions whose linear combination yields useful representations of molecular orbitals. The linear combination of basis functions, which generate molecular orbitals, is called basis set.

Slater functions (equation 2.5.) are good approximations to atomic wave functions, but large computer time is required to evaluate them. Using Gaussian functions (equation 2.6.) reduce considerably the CPU time.

br) exp( a

φ (2.5.)

) br exp( a

2. METHODOLOGY _{20}

The total wave function *ψ* is expressed as a Slater determinant of spin orbitals α and β

which for a system containing 2n electrons is:

2n ψ (2n)β 2n ψ (2n)α 2n ψ (2n)β 2n ψ (2n)β 2n (2n)α ψ 2 (2)β ψ ··· 2 (2)β ψ 2 (2)α ψ 2 (2)β ψ 2 (2)α ψ 1 (1)β ψ ··· 1 (1)β ψ 1 (1)α ψ 1 (1)β ψ 1 (1)α ψ (2n)! 1 Ψ n 2 2 1 1 n 2 2 1 1 n 2 2 1 1

(2.7.)

Next a brief survey of different kinds of basis sets is given.

*STO-nG basis sets *

This kind of basis sets are characterized by the use of *n* Gaussian primitive functions for
each basis functions in which coefficients *a* and *b* (eq. 2.6.) are fitted so that they
approximate the corresponding Slater function.3 In this sense one can distinguish
between STO-3G, STO-4G or STO-6G basis sets in which three, four and six Gaussian
functions have been used, respectively.

*Split-valence basis sets *

In split-valence basis sets while core electrons are described using one single basis function, valence electrons are described by two or more basis functions. In the present thesis two kinds of split-valence basis sets have been used: Pople basis sets and Dunning basis sets. Split-valence double-zeta Pople basis sets nomenclature follows the

with small values of coefficient *b* of equation 2.6., are recommended to be used to study
molecules with heteroatoms, anions and electronically excited molecules. Diffuse
functions are denoted with a plus sign (+) when they added only to heavy atoms and
with two plus signs (++) when they are also added to helium and hydrogen atoms.

Dunning basis sets, also called correlation consistent basis sets, are constituted by
adding shells of functions to a core set of atomic Hartree-Fock functions. Each function
in a shell contributes approximately the same amount of correlation energy. Dunning
basis sets follow the nomenclature *cc-pVXZ*, being X the degree of polarization. The
addition of diffuse functions to Dunning basis sets is denoted with the prefix “aug”.6

**2.2.3.** **Closed-shell and open-shell systems **

Closed-shell systems are those where all orbitals are doubly occupied. In other words, all electrons are split in pairs and, in each pair, electrons have opposite spins and occupy the same spatial orbitals. These systems can be handled by using the so called restricted methods, which use a single molecular orbital twice (one multiplied by the α spin function and the other multiplied by the β spin function) in the Slater determinant (eq. 2.7.).

Conversely open-shell systems are those where some of the electrons are unpaired, leading to singly occupied molecular orbitals. These systems can be treated by using unrestricted methods, which use different orbitals for different spins.

**2.2.4.** **Ab initio calculations **

2. METHODOLOGY _{22}

obtained by varying iteratively the weighting coefficients of the atomic orbitals (*csi* in

eq. 2.4.) until the energy expectation value, *E(ψ)*, of the approximate wave function is
minimized.

###

ψ ψ ψ Hˆ ψ ψE (2.8.)

The major weakness of HF method is the fact that it does not describes electron correlation properly since each electron is considered to move in an electrostatic field whereas in reality electrons repeal each other. This deficiency makes HF method not reliable to get accurate estimates of systems where electron correlation plays an important role such as π-stacking interactions or chemical reactions. Post-HF methods correct the aforementioned deficiency. In this thesis two post-HF methods have been used: Møller Plesset (MP) procedure8 and Coupled Cluster (CC) method.9 Møller Plesset is based on perturbation theory. The philosophy behind MP methods is that a correction term handles electron correlation by promoting electrons from occupied to virtual molecular orbitals giving electrons more room to move and thus making it easier for them to avoid one another. The Hamiltonian operator is defined as the addition of a

perturbation operator (*V*ˆ ) to the unperturbed HF Hamiltonian (* _{H}*ˆ0

_{): }

Vˆ

λ

Hˆ

Hˆ_{} 0 _{} _{} _{ } _{ (2.9.) }

where λ is a dimensionless parameter taking values compressed between 0 and 1. Thus both wavefunction and energy are described by this perturbed Hamiltonian operator.

(n) n (2)

2 (1)

(0) _{λ} _{ψ} _{λ} _{ψ} _{...} _{λ} _{ψ}

ψ

ψ (2.10.)

(n) n (2)

2 (1)

(0) _{λ} _{E} _{λ} _{E} _{...} _{λ} _{E}

E

E (2.11.)

The Coupled Cluster method expresses the correlated wave function as a sum of the HF ground state determinant plus determinants representing the promotion of electrons to virtual molecular orbitals:

HF
Tˆ
HF
n
3
2
ψ
e
ψ
n!
Tˆ
3!
Tˆ
2!
Tˆ
Tˆ
1
ψ _{}

_{} (2.12.)

where *T*ˆ *T*ˆ_{1} *T*ˆ_{2} _{}*T*ˆ_{n} and the operators *T*ˆ are excitation operators and have the _{n}

effect of promoting n electrons into virtual spin orbitals. In the present thesis CCSD(T) has been employed, that means coupled cluster singles, doubles and triples method being the contribution of triple excitations represented in an approximate way.

**2.2.5.** **Semiempirical calculations **

Semiempirical (SE) methods are based on the Schrödinger equation (eq. 2.1.) and
experimental data. In spite of being computationally cheaper than *ab initio* methods a
very accurate parameterization is needed to get reliable results. The main differences
between SE and *ab initio *methods lie basically in four points:

SE methods treat only valence or π electrons

The basis functions correspond to atomic orbitals while in *ab initio* calculations
this is only true when minimal basis set are used,* i.e.* the smallest number of
functions that can accommodate all the electrons.

Both core and the two electron repulsion integrals are not calculated from first principle but using empirical data.

Simplifications in the mathematical model by assuming some matrices as unit matrices.

2. METHODOLOGY _{24}

**2.2.6.** **Density Functional Theory calculations **

The Density Functional Theory (DFT) is based on the theorems of Hohenberg-Kohn12
which state that the ground state energy of a non degenerate electronic system as well as
its electronic properties are solely defined by its electron density. In consequence DFT
does not use the wave function but an electron probability density function *ρ(x,y,z)*,
which refers to the probability of finding an electron in a volume element *dxdydz*

centered on a point with coordinates (x, y, z). Assuming *r* as the position vector of the
point with coordinates (x, y, z) and taking into account Born and Pauli interpretation,
which states that the square of a one electron wave function (Kohn-Sham orbitals, ψi in

eq. 2.13.) at any point is the probability density at that point, electron density can be written as follows:

###

n 1 i (r) i ψ r) (ρ 2 (2.13.)

where *n* is the number of occupied molecular orbitals. Electronic energy *E(ρ)* is
calculated as a simple sum of different contributions that depend on the electronic
density:
)
(ρ
E
)
(ρ
E
)
(ρ
E
)
(ρ
E
)

E(ρ _{} T _{} V _{} J _{} XC _{ (2.14.) }

being *ET(ρ)* the kinetic energy, *EV(ρ)* the term containing the potential attractive energy
electron-nucleus and the repulsive term between nuclei,* EJ(ρ)* the Coulombic repulsion
between electrons and *EXC(ρ)* the interchange-correlation energy. The latest term is the
only one that is not determined directly because of its unknown mathematical
formulation. Usually *EXC(ρ)* is described as a sum of an exchange term *EX(ρ)* and
another of electronic correlation *EC(ρ)*.

) (ρ E ) (ρ E ) (ρ

EXC _{} X _{} C _{ (2.15.) }

The exchange term can be calculated by using approximations that applies a
homogeneous electron density, such as the Local Density Approximation (LDA)13 and
the Local Spin Density Approximation (LSDA),14 or by using gradient corrected
functionals such as the so called Generalised Gradient Approximation (GGA) methods.
Examples of functionals using a homogeneous electron density are the VWN15_{ or the }

reported such as Becke95 (B95), Perdew 86 (P), Perdew-Burke-Ernzerhof (PBE), Perdew-Wang 91 (PW91)20 and the extremely popular Lee-Yang-Parr (LYP).21 The exchange-correlation term can also be calculated using the so called hybrid density functionals, which combine a conventional GGA method with a percentage of Hartree-Fock exchange. Examples of hybrid density functionals include B3LYP,21,22 B3PW91,20,22 MPW1K,23 O3LYP21,24 and X3LYP.20,21,25

**2.2.7.** **Solvent effects **

Solvent effects in QM calculations have been evaluated by means of continuum models,

*i.e.* while the solvent is described as an infinite dielectric medium the solute is treated at
the QM level. In the present thesis the so called Polarizable Continuum Model (PCM)
has been employed.26 PCM is a Self Consistent Reaction Field (SCRF) method, *i.e.*

implies the use of a reaction potential to be self-consistently solved together with the solute charge.

PCM method involves the generation of a solvent cavity from spheres centered at each atom of the molecule and the calculation of virtual point-charges on the cavity surface representing the polarization of the solvent. The magnitude of these charges is proportional to the derivative of the solute electrostatic potential at each point calculated from the molecular wave function.

Within PCM method the transfer of a given solute from the gas phase into solution can be portioned into three steps:

Creation of the solute cavity inside bulk solvent.

Generation of the van der Waals particle inside the cavity. Generation of the solute charge distribution in solution.

Thus the net molecular free energy of a system in solution (*∆Gsolv*) is the sum of these

three contributions:

elec vdW

cav

solv ΔG ΔG ΔG

ΔG (2.16.)

where *∆Gcav* is the work involved to increase the cavity, *∆GvdW* is the contribution due

to the van der Waals interactions and *∆Gelec* is the electrostatic component of the ∆Gsolv

2. METHODOLOGY _{26}

perturbation operator (*V*ˆ ). Thus the Schrödinger equation, being _{R}* _{H}*ˆ0

_{ the solute’s }

Hamiltonian operator, is expressed as follows:

###

Hˆ0_{}Vˆ

_{R}

###

ψ_{}Eψ

_{ }

_{ (2.17.) }

**2.3.Molecular dynamics simulations **

Molecular dynamics (MD) simulations reproduce the dynamical evolution of a system at a molecular level by means of MM. MM methods are based on mathematical models that assume a molecule as a collection of balls and springs representing respectively atoms and bonds. Each particle is described by a radius, hardness and net charge.

**2.3.1.** **Force-Field **

Force-field (FF) is the form of the mathematical expression and the parameters needed to calculate the potential energy of a system under the MM formalism. FF includes terms referring to both bonding and non-bonding interactions. In the present thesis AMBER FF has been employed.27

###

###

###

###

###

ji o ij j i j

i ij6 ij 12 ij ij bonds dihedrals torsion angles 2 eq bend 2 eq stretcht r 4π q q r B r A γ)] cos(n [1 k ) θ (θ k ) r (r k E(r) (2.18.)

As can be seen in equation 2.18. total energy has five terms which are, respectively:
The bond stretching term in which the stretching force constant (*kstretch*) and the

distance between two bonded atoms and its equilibrium bond distance (*r* and *req*

respectively) are included.

The angle bending term including the bending force constant (*kbend*) and the

angle between three consecutive atoms and its equilibrium value (*θ* and *θeq*).

The torsional term contains a dihedral constant (*ktorsion*) setting the energy barrier

for the rotation profile, the actual dihedral angle () and the equilibrium one (*γ*).
The van der Waals non bonded term, a mathematical model following the

Lenard-Jones potential that takes into account the attractive and repulsive forces
between two atoms being the *rij* the distance between them. *Aij* and *Bij* are

parameters that depend of the pair of atoms referring to hard core repulsion and dispersive attraction respectively.

The electrostatic interactions are taken into account in the last term, where *qi*and

*qj* are the point charges of atoms *i* and *j* respectively, *rij* is the distance between

2. METHODOLOGY _{28}

All the constants in 2.18. as well as all the equilibrium values are taken from AMBER
libraries. All the terms not found in such libraries must be parameterized either using
experimental data or by means of *ab initio* or DFT calculations. In the present thesis
charges have been obtained from QM *ab initio *calculations according to either the
so-called Restrained Electrostatic Potential (RESP)28 or by fitting the quantum mechanical
and the Coulombic Molecular Electrostatic Potential (MEP).29

**2.3.2.** **Mathematical model****of molecular dynamics **

Given an atom *i* with mass *mi* and considering that its position is described by a three

dimensional vector *ri*, its motion is ruled by Newton’s law

i
i
i
m
F
dt
)
(
dv
*t*
(2.19.)
dt
(t)
dr
(t)
v i

i (2.20.)

where *vi*and *Fi* are respectively the velocity and the force acting on the atom *i *in a given

moment. *Fi* can be obtained through equation 2.21.

i N i r ) E(r F

(2.21.)

where *E(rN)* is given by eq. 2.18. and *N* is the number of particles in the system.

Equations 2.19. and 2.20. form a system of *N* coupled differential equations that might
be solved numerically. This system can be integrated step by step by the so called
leap-frog Verlet algorithm,30 which is founded on a Taylor expansion of the position *ri* at

time *tn=t0+n∆t*, leading to equations 2.22. and 2.23.

###

3 i N i n i ni oΔt

r
)
E(r
m
Δt
2
Δt
t
v
2
Δt
t
v
_{}

_{} _{ }_{(2.22.) }

###

###

###

4n i n i n

i Δt oΔt

2 Δt t v t r Δt t

r

_{}

(2.23.)

values of the order of the femtosecond. Small time steps lead to more expensive simulations.

The CPU time needed for a MD simulation depends on several factors as the number of
the explicit particles in the system, the time step or the cut-off, *i.e.* the maximum
distance in which non bonded interactions are evaluated. In order to speed up the MD
simulation some simplifications might be done such as freezing the fastest modes of
vibration by constraining the bonds to hydrogen atoms to fixed lengths. In this sense,
SHAKE or constrained Verlet method31 has been used in this thesis.

**2.3.3.** **Thermodynamic ensembles **

An ensemble is a collection of all possible systems that have differing microscopic states but belong to a single macroscopic or thermodynamic state. There are four ensembles that are used in MD simulations.32

The canonical or NVT ensemble, whose thermodynamic state is characterized
by a fixed number of atoms *N*, fixed volume *V* and fixed temperature *T*.

The isobaric-isoenthalpic or NPH ensemble, where the number of atoms *N*, the
pressure *P* and enthalpy *H* are fixed.

The isobaric-isothermal or NPT ensemble, with fixed values of number of atoms

*N*, pressure *P* and temperature *T*.

The microcanonical or NVE ensemble, which corresponds to a closed or isolated
system since energy *E*, besides the number of atoms *N* and volume *V*, is fixed.
In the present thesis NVT and NPT ensembles have been employed. Temperature is
mainly set by the average kinetic energy of the molecules of the system. Consequently
temperature can be controlled by adjusting the velocities of each atom. Berendsen
thermostat rescales velocities of atoms assuming a scale factor *λ* defined as:

2
1
0
1
1 _{}
*T*
*T*
*t*
*T*

(2.24.)

where *τT* is the heat bath coupling time and *T0*is the set point temperature. Concerning

2. METHODOLOGY _{30}

###

###

31

0 P

P P

τ Δt 1

μ _{}

(2.25.)

where *τP* is the pressure relaxation time of the barostat and *P0* is the set point pressure.

Equations 2.24. and 2.25. define the so called Berendsen thermobarostat.33

**2.3.4.** **Periodic boundary conditions and Particle Mesh-Ewald Summation **

**2.4.QM/MM calculations **

QM/MM methods are based in splitting the system in two parts, a small one of special interest described at the QM level and the rest of the system described at the MM level. QM/MM philosophy was firstly introduced by Warshel and Levitt35 and developed by Field, Bash and Karplus.36 QM/MM methods differ, besides the classical force field and the QM level of theory employed, in how the two parts are connected. There are two way to connect QM and MM parts:

The so called link atom scheme, which uses a monovalent atom to cap the unsaturated QM atoms. Normally hydrogen atom is used as link atom.37

Methods based in the use of localized orbitals in the boundaries separating the QM and MM parts. One example is the Local Self-Consistent Field (LSCF) method38 in which the bonds connecting both parts are represented by a set of strictly localized bond orbitals (SLBOs) that are determined by calculations on small model compounds and assumed to be transferable.

Within the framework of QM/MM calculations the total Hamiltonian operator is defined as the sum of the QM, QM/MM and MM Hamiltonians:

MM QM/MM

QM _{Hˆ} _{Hˆ}

Hˆ

Hˆ (2.26.)

where * _{H}*ˆ

*QM*/

*MM*

_{is expressed as the sum of electron-charge, nuclei-charge and van der }Waals interaction potentials between QM and MM atoms:

QM/MM vdW QM/MM nucl QM/MM elec

QM/MM _{V} _{V} _{V}

Hˆ (2.27.)

Equation 2.27. can be expanded for a system containing *N* QM atoms and *M* MM atoms
as follows:

###

###

###

###

N 1 i N 1 i M 1j ij6 ij 12 ij ij N 1 i M 1 j ij j i M 1 j ij j QM/MM r B r A r q Z r q

Hˆ (2.28.)

Thus energy in a QM/MM system is defined as shown in Equation 2.29.

QM/MM MM

QM _{E} _{E}

E

2. METHODOLOGY _{32}

where * _{E}QM*/

*MM*

_{is defined as: }

QM/MM vdW QM/MM

nucl N

1 i

M 1 j ij

j

QM/MM _{ψ} _{V} _{V}

r q

ψ

E

###

(2.30.)

where the first term is the electronic interaction within the Electronic Emboding scheme.

.

**2.5.References **

[1] Lewars E. “Computational Chemistry: Introduction to the Theory and Applications
of Molecular and Quantum Mechanics”, **2004**, Kluwer Academic Publishers, Dordrecht.
[2] a) Roothaan C.C.J. *Rev. Mod. Phys.* **1951**, *23*, 69. b) Hall G.G., *Proc. Roy. Soc.*
**1951**, *A205*, 541.

[3] Hehre W.J., Stewart R.F., Pople J.A. *J. Chem. Phys.***1969**, *51*, 2657.
[4] Binkley J.S., Pople J.A., Hehre W.J. *J. Am. Chem. Soc.***1980**, *102*, 939.
[5] Ditchfield R., Hehre W.J., Pople J.A. *J. Chem. Phys.***1971**, *54*, 724.

[6] a) Dunning T.H. *J. Chem. Phys.* **1989**, *90*, 1007 b) Kendall R.A., Dunning T.H.,
Harrison R.J. *J. Chem. Phys.* **1992**, *96*, 6796 c) Woon D.E., Dunning T.H. *J. Chem. *
*Phys.***1993**, *98*, 1358 d) Peterson K.A., Woon D.E., Dunning T.H. *J. Chem. Phys.***1994**,

*100*, 7410 e) Wilson A., van Mourik T., Dunning T.H. *J. Mol. Struct. (Theochem)***1997**,

*388*, 339.

[7] a) Hartree D.R. *Proc. Cambridge Phil. Soc.* **1928**, *24*, 89 b) Slater J.C. *Phys. Rev.*
**1930**, *35*, 210 c) Fock V. *Z. Physik***1930**, *61*, 126.

[8] a) Møller C., Plesset M.S. *Phys. Rev.***1934**, *46*, 618 b) Binkley J.S., Pople J.A. *Int. J. *
*Quantum Chem.*, **1975**, *9*, 229.

[9] a) Coester F., Kümmel H. *Nucl. Phys.* **1960**, *17*, 477 b) Paldus J., Čížek J. Shavitt I.

*Phys. Rev. A ***1972**, *5*, 50.

[10] a) Stewart J.J.P. *J. Comp. Chem. ***1989**, *10*, 209 b) Stewart J.J.P. *J. Comp. Chem. *
**1989**, *10*, 221 c) Stewart J.J.P. *J. Comp. Chem.***1991**, *12*, 320.

[11]Dewar M.J.S., Zoebisch E.G., Healy E.F., Stewart J.J.P. *J. Am. Chem. Soc.* **1985**,

*107*, 3902.

[12] Hohenberg P., Kohn W. *Phys. Rev. B ***1964**, *136*, B864.
[13] Slater J.C. *Int. J. Quantum Chem. Symp.***1975**, *9*, 7.
[14] Painter G.S. *Phys. Rev. B ***1981**, *24*, 4264.

[15] Vosko S.H., Wilk L., Nusair M. *Can. J. Phys.***1980**, *58*, 1200.
[16] Perdew J.P., Zunger A. *Phys. Rev. B***1981**, *23*, 5048.

[17] Becke A.D. *J. Chem. Phys.***1996**, *104*, 1040.
[18] Perdew J.P. *Phys. Rev. B***1986**, *33*, 8822.

[19] Perdew, J.P., Burke, K., Ernzerhof M. *Phys. Rev. Lett.***1996**, *77*, 3865.
[20] Perdew J. P., Wang Y. *Phys. Rev. B***1992**, *45*, 13244.

2. METHODOLOGY _{34}

[22] Becke A.D. *J. Chem. Phys.***1993**, *98*, 1372.

[23] a) Adamo C., Barone V. *J. Chem. Phys.* **1998**, *108*, 664 b) Lynch B.J., Fast P.L.,
Harris M., Truhlar D.G. *J. Phys. Chem. A* **2000**, *104*, 4811 c) Lynch B.J., Zhao Y.,
Truhlar D.G. *J. Phys. Chem. A***2003**, *107*, 1384.

[24] Schultz N.E., Zhao Y., Truhlar D.G. *J. Phys. Chem. A***2005**, *109*, 11127.

[25] a) Becke A.D. *Phys. Rev. A* **1988**, *38*, 3098 b) Xu X., Goddard W.A. *Proc. Natl. *
*Acad. Sci. U.S.A.***2004**, *101*, 2673.

[26] a) Miertuš S., Scrocco E., Tomasi J. *Chem. Phys.* **1981**, *55*, 117 b) Miertuš S.,
Scrocco E., Tomasi J. *Chem. Phys. ***1982**, *65*, 239.

[27] a) Cornell W.D., Cieplak P., Bayly C.I., Gould I.R., Merz K.M., Ferguson D.M.,
Spellmeyer D.C., Fox T., Caldwell J.W., Kollman P.A. *J. Am. Chem. Soc. ***1995**, *117*,
5179 b) Wang J., Cieplak P., Kollman P.A. *J. Comput. Chem. ***2000**, *21*, 1049.

[28] a) Bayly C.I., Cieplak P., Cornell W., Kollman P.A. *J. Phys. Chem.***1993**, *97*,
10269 b) Cornell W.D., Cieplak P., Bayly C.I., Kollmann P.A. *J. Am. Chem. Soc.***1993**,

*115*, 9620.

[29] Alemán C., Luque F.J., Orozco M. *J. Comput. Aided Mol. Design***1993**, *7*, 721.
[30] Verlet J. *Phys. Rev.***1967**, *159*, 98.

[31] a) van Gunsteren W.F., Berendsen H.J.C. *Mol. Phys.***1977**, *34*, 1311 b) Ryckaert J.
P., Ciccotti G., Berendsen H.J.C. *J. Comput. Phys.***1977**, *23*, 327.

[32] Adcock S.A., McCammon J.A. *Chem. Rev.***2006**, *106*, 1589.

[33] Berendsen H.J.C., Postma J.P.M., van Gunsteren W.F., DiNola A., Haak J.R. *J. *
*Chem. Phys.***1984**, *81*, 3684.

[34] Darden T., York D., Pedersen L. *J. Chem. Phys. ***1993**, *98*, 10089.
[35] Warshel A., Levitt M. *J. Mol. Biol.***1976**, *103*, 227.

**3.1.Testing β–helix terminal coils stability by targeted substitutions with **
**non-proteogenic amino acids: A Molecular Dynamics study***

**3.1.1.** **Introduction **

An important aim of nanotechnology is to design new microscopic devices at the
molecular level, necessitating the tuning of the structural and physicochemical features
of its molecular parts. An increasingly common strategy is to combine polymer science
with advanced organic synthesis procedures.1 Nanoconstructs are usually built by
assembling of macromolecular components, modules or building blocks, either via
covalent linkages or self assembly processes.2 However, detailed knowledge of the
principles that govern the organization of the nanostructures is still lacking: currently,
successful strategies are largely based on the assumption that isolated modules
inherently present an acceptable degree of ordered organization, sufficient to guarantee
and promote the correct formation of the nanoconstruct.3 This restricts the type of
building blocks that can be selected for nanodesign, since the inherent capacity for
self-organization needs to be a preferred feature. Building blocks of natural origin appear as
a logical choice in this respect, since subcellular biological structures exist and operate
at the nano scale: the molecular machinery that makes life possible is inherently based
on self assembled structures that perform specific and extraordinarily complex
functions.4_{ Creation of nano-sized structures follows the same principles that control the }

folding and the stability of interacting biomolecules.5 Whether in natural structures or in nanoconstructs, the final product is the last stage in a hierarchical chain of chemical events that initiate with the selection of those building blocks with molecular conformations that favor a particular assembly.6 In such a scheme, the stabilization of conformational motifs of natural building blocks extracted from their natural environment, is an important task.

In recent years the use of segments extracted from proteins as molecular scaffolds to build tubular nanoconstructs has been explored.7 For this purpose, several efforts have been centered on the β–helix fold: a conformational arrangement that contains a repetitive helical strand-loop motif, where each repeat contributes a strand segment to one or more parallel β sheet(s). Systems containing left-handed β-helical building blocks are of special interest since this arrangement is highly repetitive and

** **

3. NANOTUBES BASED ON NATURAL PEPTIDE SEQUENCES _{40}

symmetrical, which should allow the formation of nanofibers without performing many
structural manipulations.8 As compared with right-handed β-helices, left-handed β
-helices exhibit limited variability of shape, size and sequence,9 displaying the
characteristic equilateral triangular shape. It was demonstrated that the nanofibril
constructed by four stacked replicas of a two-turn repeat building block (i.e. a β-helix
terminal coil) from the *Escherichia coli* galactoside acetyltransferase (PDB code 1krr,
chain A) exhibits remarkable stability under different simulation conditions, including
temperature stress and various ionic strengths.7 Results indicated that the formation of a
nanofibril by self-assembling is granted if the native conformation of the building block
is preserved once it is excised from the whole protein. Yet, this necessary condition is
difficult to accomplish, since even in the best scenario, the desired conformation would
only be part of a set of conformers that define the structure of the building block in
solution.

Previous contributions toward the engineering of nanotubular architectures was to shift
the population balance toward the desired conformation by selective stabilization of key
positions along the peptide chain.7,10 The conformational preferences of the building
blocks, extracted from whole β-helix proteins were first probed *in silico*; next, positions
observed to be most sensitive to conformational disorder were stabilized. This was
accomplished by replacing the chosen positions by synthetic amino acids with restricted
conformational space.10 To date, the most flexible regions of the β-helix capping coil,
the turns, have been the replacement targets since such substitutions would contribute
substantially to destabilize the whole conformation. Overall, the results of these
investigations have confirmed this assumption.7,10 However, in some cases the
connection between the β-sheet segments becomes too rigid if the flexibility of the loop
is reduced.10b An alternative approach would be to fix the β-sheet segments by targeted
replacements; however, without altering the flexibility of the loop.

In order to choose the proper target sites for the stabilization of the β-sheet segments in the wild type sequence, some previous considerations were taken into account:

(ii) The targeted position should preferably be in the center of the β-sheet to avoid undesirable conformational influence in the adjacent loops;

(iii) The residue type should preferably be hydrophobic, since polar groups may induce competitive interactions with other side chains destabilizing the whole motif more easily than hydrophobic side chains, due to the lager range of action of polar interactions;

(iv) The size of the targeted side chain should be voluminous enough to allow the replacement by a conformationally restrained amino acid, which is quite large. Thus, conformational restrictions are usually introduced by modifying the main chain or the side chain of conventional α-amino acids.

In this chapter the investigated system is the aforementioned protein segment excised
from the chain A of *E. coli* galactoside acetyltransferase, which comprises residues
131-165, hereafter referred to solely as 1krr. If the considerations exposed above are applied
to 1krr, the most suitable positions to be target for replacement are the valines in
positions 145 and 157 (Figure 1). These residues, located in the middle of their
respective β-sheets, do not project inward, toward the helix inner cavity; hence,
reducing the hydrophobicity of the site may be expected to increase the sheet solubility
and, therefore, the conformational stability.

**Figure 1.** Equatorial (top) and axial (bottom) partial
projections of the -helical building block extracted for
the crystal structure of 1krr131-165segment. The motif is

3. NANOTUBES BASED ON NATURAL PEPTIDE SEQUENCES _{42}

Six different synthetic amino acids have been tested as possible stabilizing agents (Scheme 1). These series were chosen because they are relatively easy to synthesize, their conformational properties have already been characterized (in most cases both theoretically and experimentally) and in most cases have already been used in conformational studies of polypeptides (see below for details).

**Scheme 1 **

On the other hand, although the conformational properties of three of them are more restricted than those of proteogenic residues, the characteristic shared by all the amino acids probed is the ability to favor extended or pseudoextended conformations under proper conditions. At the same time, it was attempted to cover a broad range of chemical modifications that can be introduced into proteonogenic amino acids, which justifies the variability of the tested amino acids.

The results presented in this work clearly demonstrate that the stability of -helix terminal coils is extremely site sensitive, which implies that the conformational properties of the amino acids are not the sole determinants in enhancing the stability of peptide segments folded in -sheets. This is illustrated by the fact that only when the conformational alteration induced by the synthetic amino acids is combined with the formation of new mid- and long-range interactions, the overall stability of the -helix capping coil can be enhanced. In spite of the steric hindrance imposed by the voluminous phenyl side chains, diphenylglycine (Dg) has been found to be the best option for the enhancement of the building block stability. This is because the side

N C C H O C H H N C C H O N C C H O CH3 CH3 N CH2 CH2 C H O N C C H O

CH CH3

CH3 N C C H O CH3

**Ala** **Ala** **Aib** **D****g**

**D-Ala**
**D-Val**
N
C
C
H O
C
H H
N
C
C
H O
N
C
C
H O
CH3
CH3
N
CH2
CH2
C
H
O
N
C
C
H O

CH CH3

CH3 N C C H O CH3

**Ala** **Ala** **Aib** **D****g**

chains form new non-covalent interactions with neighboring residues, which provides rigidity to the –sheet segments in the fold.

**3.1.2.** **Survey of Synthetic Amino Acids **

Four synthetic amino acid types, which differ significantly in their chemical constitution, have been considered for targeted replacements. This section describes the more important characteristics of each amino acid type.

*Dehydroalanine (**Ala)*

This is an ,-unsaturated amino acid commonly found in a number of naturally occurring peptide antibiotics of bacterial origin.11 The conversion of the tetrahedral saturated to a trigonal dehydro residue with a shortening of the C-C distance introduces strong and specific steric effects, which influence its conformational behavior. Thus, the double bond of the side chain enhances the stability of the extended and (pseudo)extended conformations in both single residues.12

*-Dialkylated amino acids: **-aminoisobutyric acid (Aib) and diphenylglycine (D**g) *

Substitution of the -carbon hydrogen by an alkyl group induces drastic changes in the conformational properties of amino acids, which are frequently associated with the incorporation of strong conformational constraints. The simplest -amino acid is Aib, in which a methyl group replaces the -carbon hydrogen of Ala, while Dg should be considered as a Gly derivative with two bulky phenyl groups replacing the corresponding -carbon hydrogen atoms. It was recently found that Dg prefers an extended conformation,13 although depending on the peptide sequence, it can also be part of helix arrangements, such as 310 helix organization.14 In contrast, Aib promotes

folded conformations,15 hence this residue is used in this work for comparison with Dg.

*-Alanine (**Ala)*